Biosorption of lead by the brown seaweed Sargassum filipendula - batch and continuous pilot studies
Carlos Augusto da Costa
Pessôa de França*
Keywords: biosorption, biosorption equilibrium, continuous system, lead, Sargassum filipendula.
The biosorption of lead by the
brown alga Sargassum filipendula was studied. pH 4.0 was the
optimum value for the biosorption of lead. Isotherms indicated that
for solutions containing 0.03 ± 0.001 up to 3.27 ± 0.04 mmol/L of
lead, 2.0g/L was the optimum biomass concentration. The Langmuir model
was fitted to represent the experimental data, and the kinetics of
biosorption presented equilibrium in 30 min. The continuous system
operated for 56 hrs presenting a 100% binding of ionic lead, which
corresponds to an accumulation of
Industries that work with car batteries, sheets of semifinished metal, additives in gasoline, ammunition and scrap iron from car batteries are the main sources of effluents containing lead. Besides respiratory problems, lead provokes alterations in blood and urinary system.
is a brown seaweed typically found in tropical countries and abundant
in South America, and it is easily collected on beaches without any
environmental damage due to its occurrence/presence in the tropical
The main polysaccharide in Sargassum seaweed is alginic acid, a polymer containing β-1,4 manuronic acid (M) associated to α-1,4 guluronic acid (G). The M/G content in different brown seaweeds may vary under different environmental conditions and with different species, with both monomers able to accumulate heavy metals.
Literature presents few examples of the continuous application of biosorption, most of which are focused on surveys on operational parameters for selected systems. Volesky et al. (2003) tested a fixed-bed column reactor, filled with Sargassum filipendula, for the recovery of ionic lead, emphasizing the desorption of metal and the hydraulic conditions of the continuous system.
Sargassum sp. biomass was used in the recovery of ionic copper
from highly concentrated solutions simulating effluents from semiconductor
production. The continuous system used contained four column reactors
filled with the biomass of Sargassum sp. and showed high operational
stability. Biomass of Sargassum sp. in the reactors was gradually
saturated from the bottom to the top of each column reactor. The biomass
of Sargassum sp. in the first column was saturated first, followed
by a gradual saturation of the remaining columns due to the pre-concentration
caused by the biomass in the first column. The biomass of Sargassum
in the bioreactors completely biosorbed the ionic copper contained
The zinc biosorptive capacity of the brown seaweed Sargassum sp. (Phaeophyceae) was studied in the presence or absence of competing calcium ions, using a continuous system with tubular fixed-bed reactors (de França et al. 2002). In order to detect the effect of calcium on zinc biosorption, a 130 mg/L zinc solution was used, and calcium was added at 50-340 mg/L. The potential zinc biosorptive capacity of the biomass was markedly influenced by the presence of ionic calcium. Zinc sorption decreased with increasing calcium concentrations, as expressed by zinc uptake rates. Calcium was effectively recovered only during the initial stages of the process, as expressed by the decrease in its uptake rates. Calcium uptake rates were also much higher than zinc uptake rates, indicating that calcium was preferentially recovered when compared to zinc.
Biosorption of Pb(II) and Cu(II) ions in single component and binary systems was studied using activated sludge in continuous-flow stirred reactors. Because of the low adsorption capacity of the non-viable activated sludge especially in the case of Pb(II) ions, biosorption of the Cu(II) and Pb(II) ions from the binary mixtures was carried out by using the resting cells. The biosorption data fitted better with the Freundlich adsorption isotherm model. Using a mathematical model based on continuous system mass balance for the liquid phase and batch system mass balance for the solid phase, the forward rate constants for biosorption of Pb(II) and Cu(II) ions were 0.793 and 0.242 (mmol/min), respectively (Sag et al. 2003).
This research aimed to study the biosorption of lead by Sargassum filipendula in batch and continuous systems, obtaining equilibrium parameters in a static system to aid in the dynamic operation of bioreactors for the treatment of ionic lead in high concentrations.
Sargassum filipendula (Phaeophyceae,
Cyclosporeae, Fucales, Sargassaceae) was the biosorbent material.
The biomass was obtained from the Northeastern coast of
filipendula was washed with distilled water and oven-dried at
investigate the optimum pH for the biosorption of lead by S. filipendula,
pH values of lead nitrate solutions (0.23 ± 0.01 mmol/L) were adjusted
to 4.0, 4.5 and 5.0. These tests were performed in the absence of
the biomass and with the addition of S. filipendula (2.0 g/L).
The pH was monitored before and after the equilibrium, to differentiate
chemical precipitation and biosorption. Experiments were performed
in a shaker, at 150 rpm and 30 ±
these experiments, 50 mL of lead nitrate in the concentrations of
0.03 ± 0.001 to 3.27 ± 0.04 mmol/L at pH 4.0 were incubated in a shaker
for 24 hrs at 30 ±
The lead uptake (Q) was calculated by the simple concentration difference method. The initial concentration, C0 (mg/L), and the metal concentration at any time, Ct (mg/L), were determined. Metal uptake Q (mmol lead/g S. filipendula) was calculated from the mass balance (1):
where V is the volume of solution (mL) and w the mass of sorbent (g).
The obtained experimental data were fitted to Langmuir and Freundlich equations, which are the most widely used in biosorption (Cossich et al. 2002; Cruz et al. 2004). The Langmuir model assumes the form (2):
where Q0 (mmol/g) is the maximum amount of metal ion per unit weight of algae to form a complete monolayer on the surface. Ce (mmol/L) corresponds to the equilibrium concentration and KL (L/mmol) is the equilibrium adsorption constant, related to the affinity of the binding sites. Q0 represents the limiting adsorption capacity for adsorption performance (Aksu, 2001). Parameters can be determined from a linearized form of (2), represented by (3):
A plot of (Ce/Qe) versus Ce, gives a straight line of a 1/Q0 slope and a 1/(Q0KL) intercept. On the other hand, the Freundlich equation is given by (4):
Qe = KF (Ce)1/n 
where KF and n are the Freundlich constants, indicating the adsorption capacity and adsorption intensity, respectively. The derivation of KF and 1/n, can be linearized in logarithmic form (5):
logQe = log KF + (1/n) log Ce 
For the kinetic study of the biosorption of lead by S. filipendula, the concentration of ionic lead was monitored throughout the time (up to 45 min), using a solution containing lead in the concentration of 0.23 ± 0.01 mmol/L, at pH 4.0.
continuous system contained four serial fixed-bed column reactors,
Five experiments were conducted in a continuous system, each of them at a distinct concentration: 0.24 ± 0.02, 0.48 ± 0.05, 1.21 ± 0.10, 2.42 ± 0.23 and 4.83 ± 0.62 mmol/L ionic lead, at pH 4.0. Samples were collected from the top of each column at three-hour intervals, filtered, acidified and quantified in relation to the lead content. Each experiment was conducted during 60 hrs and repeated four times under the same conditions; therefore, the reported values constitute the average lead determinations for each experimental condition. Standard deviations were calculated to estimate the dispersion levels of the individual values in relation to a calculated mean value.
Through each breakthrough curve that was obtained, it was possible to evaluate the performance of the continuous system, thus identifying the most adequate operational conditions.
The biosorption of lead by S. filipendula at different pH values is presented in Table 1.
The presented results indicate that in the absence of the biomass a chemical precipitation occurred since the lead began to precipitate after pH 4.5. At pH 5.0, however, the chemical precipitation was the most pronounced in relation to the values at pH 4.0 and 4.5.
In the experiments in which the biomass was added, the equilibrium concentrations of lead were considerably lower in comparison to the chemical precipitation, which indicates a great contribution of the biosorption in relation to the chemical precipitation.
The equilibrium concentrations ranged from 0.002 to 0.005 mmol/L, crescent in relation to the pH increase. At pH lower than 3.0, lead removal was inhibited possibly as result of a competition between hydrogen and lead ions, with an apparent preponderance of hydrogen ions. For this reason those results are not reported in Table 1. With an increase in pH, the negative charge density on the biomass increases due to deprotonation of the metal binding sites, thus increasing metal biosorption.
The pH is one of the most important parameters of biosorption (Kapoor et al. 1999; Aksu, 2001) and, regarding Sargassum sp., its high content of ionizable groups (carboxyl groups), makes it very liable to be influenced by the pH of the medium. For Sargassum sp., carboxyl groups are chiefly responsible for binding metallic ions.
However other functional groups may contribute to the process, such as the sulfonate and amine groups.
The higher the pH value, the higher the dissociation since free sites for the binding of lead can be produced, however, the majority of heavy metals precipitate at pH values over 5.5.
Ho (2005), using tree fern, showed that pH values in the range of 4.0 to 7.0 were adequate for lead binding, of which pH 4.9 is the optimum value for the biosorbent.
These values are contrary to those obtained in the present research, the aim of which was the preponderance of chemical precipitation.
Associating the fact that at pH 4.0 no chemical precipitation occurred to the fact that the lowest equilibrium concentration was obtained, this value was considered ideal for subsequent experiments.
The results that were obtained through batch processing are presented in Figure 1. Evaluating the results presented in Figure 1, it can be concluded that for the concentrations in the range of 0.03 ± 0.001 to 3.27 ± 0.04 mmol/L, under the conditions of the experiments, a biomass concentration equal to 2.0 g/L was the most interesting since it generated the lowest equilibrium concentrations.
An analysis of Figure 1 can be carried out not only considering the obtained equilibrium concentrations for the different lead solutions, but also evaluating its uptake capacity.
For all biomass concentrations tested, the uptake capacities increases with the equilibrium concentration, up to 0.5 mmol/L, and then tend to a constant value. Similarly, the value that was measured for the maximum uptake capacity of the biomass has not demonstrated a significant variation among the values of which the mean value was 1.2 mmol Pb/g S. filipendula.
The main difference that was observed relates to the curve profiles. In the 0.5 g/L biomass concentration, the experimental stabilization of the lead uptake by the biomass can be verified probably due to the saturation of the binding sites. However, with biomass concentrations of 1.0 and 2.0 g/L, this tendency to stabilize was not observed because these biomass concentrations could still lead to a uptake of additional ionic lead if higher lead concentrations were used.
Matheickal and Yuh (1999) reported that batch equilibrium experiments showed that the maximum adsorption of lead by chemically modified Durvillaea potatorum was 1.6 mmol/g and 1.3 mmol/g for Ecklonia radiata, which is slightly higher than the maximum value obtained in this research in the batch system (1.2 mmol/g). Raize et al. (2004) reported the binding capacities for different cations, including lead to be between 1 and 1.2 mmol metal/g on a dry weight basis.
Table 2 presents the results of Langmuir and Freundlich lead adsorption constants on Sargassum filipendula. It can be seen a good correlation between the values estimated by the Langmuir model and the experimental results (Figure 1). The maximum values for the experimental Q were 1.16, 1.14 and 1.26 mmol lead/g biomass, with 0.5, 1.0 and 2.0 g/L of S. filipendula, respectively.
The values predicted by the model based on the Langmuir equation were 1.18, 1.20 and 1.35 mmol/g, with the addition of 0.5, 1.0 e 2.0 g/L of S. filipendula, respectively. This corresponds to very small percent differences that are corroborated by the high coefficients of the obtained correlations.
From Table 2 it can be observed that the Freundlich isotherm did not fit the experimental data as good as the Langmuir model, which can be proved by the values of the corresponding constants and correlation coefficients.
The data in Table 2 indicate a low correlation between the experimental values and those estimated by the Freundlich model. The Freundlich model does not predict the surface saturation of the adsorbent after the formation of a monolayer on the metal.
The overall batch results indicate that the Langmuir isotherms best fitted the experimental data over the studied experimental range since they presented higher correlation coefficients in all of the biomass concentrations. The experimental data and the predicted profiles are in agreement in the entire range of Ce and the evaluated biomass concentrations. Jalali et al. (2002) confirmed that Sargassum hystrix, Sargassum natans and Padina pavonia removed lead efficiently from an aqueous solution, fitting Langmuir and Freundlich models and with an increasing uptake of the metal with increasing pH values.
Table 3 presents a comparison of Pb(II) sorption capacities for some conventional and biological sorbents. Those results indicate that the biosorption capacity of Sargassum filipendula biomass is just comparable to the performance observed by the marine algae Durvillaea potatorum and Ecklonia radiata (Matheickal and Yu, 1999). The remaining conventional sorbents reported and other biological materials such as the fungus Rhizopus arrhizus and the bacteria Pseudomonas aeruginosa did not present uptake capacities comparable to the values obtained in the present work.
The results that were obtained from the kinetic study of biosorption is presented in Figure 2. They indicate an extremely rapid kinetic rate of Pb(II) removal in the first min, and an approach to reach equilibrium in about 10 min. Thus, in the present work, the kinetics of lead removal was not modeled.
Other literature reports that the biosorption of metallic elements by the biomass of the brown seaweed Sargassum sp. is a rapid phenomenon; however, the time to reach equilibrium is not as short as that observed in the present work.
Jalali et al. (2002) reported that the biosorption of lead by eight types of marine algae rapidly occurred and that most of the adsorbed metal was bound in less than 30 min. Sheng et al. (2004) observed for distinct seaweeds, among which Sargassum sp. and Padinasp., a 60-min equilibrium time for lead, with an accumulation of 0.61 to 1.16 mmol/g for Sargassum sp. and 0.63 to 1.25 mmol/g for Padina sp. Likewise, Keskinkan et al. (2004) reported that the biosorption of lead by the aquatic plant Ceratophyllum demersum presented equilibrium in 20 min with an accumulation of 0.21 mmol/g.
The experiments that were carried out in the continuous system, at lead concentrations varying between 50.0 and 500.0 mg/L in the effluent, presented the total uptake of lead, thus, not reported graphically. The results of the effluents containing lead in the concentration of 1,000 mg/L (4.83 mmol/L) are presented in Figure 3.
The breakthrough curves were obtained under optimized hydraulic operational conditions. The critical bed depth, residence time and flow rate were optimized in preliminary experiments in order to observe the Brazilian Legislation as established by the National Environmental Council (CONAMA, 1986).
the curve of the first reactor of the continuous system, it can be
verified that until 12 hrs of operation, the first column removed
the loaded lead with a 100% efficiency, which corresponds to the treatment
Subsequently, a residual concentration of lead began to increase substantially related to the gradual saturation of the binding sites on the surface of S. filipendula, until reaching a value near the loading concentration, indicating saturation.
The performance of the column is related to the length and width of the absorption zone, which is developed between the section that is saturated with metal and the one that contains free biosorbent. When this adsorbent zone or mass transferal reaches the highest part of the bed, the solute in the effluent begins to increase; then, the system initiates the rupture. This point, which is called the breakthrough point is to be the maximum allowable lead concentration (0.5 mg/L).
Column 1 saturated completely after 28 hrs of continuous operation. From this point, at which the S. filipendula biomass was no longer able to remove the lead, it began to feed column 2.
the curve corresponding to the second reactor of the continuous system,
there was an effective treatment of
the fourth column of the continuous system, it can be verified that
after the treatment of
cumulative results of the continuous system demonstrate that all of
the influent lead loaded into to the system was treated, that is,
all of the lead was removed by the biomass inside the fixed-bed reactors.
Through a global evaluation, it can be concluded that
This reactor is still far from saturation with lead, which can be observed by its breakthrough curve. The system could still operate for some more hrs since the lead concentration that comes out of the fourth bioreactor, after 56 hrs of operation, is zero. The system treated all of the loaded solution and the Sargassum filipendula biomass presented, at the least, an uptake capacity of the metallic element in the order of 350 mg lead/g S. filipendula (1.70 mmol/g). It must be emphasized that the capacity of the biomass of accumulating lead can be even higher than aforementioned since the fourth reactor of the system still shows potential for higher accumulation rates of the metal.
In subsequent experiments, the biomass may be treated so as to allow the recycling of lead (Jeon et al. 2005) accumulated in its structure. Then, the first reactor of the continuous system will return to the system in the last position (as the fourth reactor) while the global system still operates. The other bioreactors may undergo similar treatment, and so continue until the biomass loses its capacity to remove the metal and needs to be substituted, as conventionally done with ion-exchange resins.
pH value that was selected for the experiments on the biosorption
of lead by S. filipendula was pH 4.0 since it combined the
best characteristics for the lowest chemical precipitation and the
highest biosorption. The Langmuir isotherms represented the batch
removal system well, achieving a maximum uptake rate of the metallic
element of 243 ± 0.04 to 277.7 ± 0.02. The rapid kinetics turns the
process attractive for the use in fixed-bed bioreactors, which can
be confirmed by the batch experiments in which the uptake time, until
reaching equilibrium, was approximately 30 min, which allowed for
a long-term operation of the continuous system. The experimental data
that were modeled into kinetic equations indicate second-order kinetics
during the biosorption. The continuous system recovered a high quantity
AKSU, Z. Equilibrium and kinetic modeling of cadmium(II) biosorption by C. vulgarisin a batch system: effect of temperature. Separation and Purification Technology, January 2001, vol. 21, no. 3, p. 285-294. [CrossRef]
CHANG, Jo-Shu; LAW, Robin and CHANG, Chung-Cheng. Biosorption of lead, copper and cadmium by biomass of Pseudomonas aeruginosa PU-21. Water Research, July 1997, vol. 31, no. 7, p. 1651-1658. [CrossRef]
CRUZ, Claudio C.V.; DA COSTA, Antonio Carlos A.; HENRIQUES, Cristiane Assumpçäo and LUNA, Aderval S. Kinetic modeling and equilibrium studies during cadmium biosorption by dead Sargassum sp. biomass. Bioresource Technology, February 2004, vol. 91, no. 3, p. 249-257. [CrossRef]
DE FRANÇA, Francisca Pessôa; TAVARES, Ana Paula and DA COSTA, Antonio Carlos Augusto. Calcium interference with continuous biosorption of zinc by Sargassum sp. (Phaeophyceae) in tubular laboratory reactors. Bioresource Technology, June 2002, vol. 83, no. 2, p. 159-163. [CrossRef]
HO, Yuh-Shan. Effect of pH on lead removal from water using tree fern as the sorbent. Bioresource Technology, July 2005, vol. 96, no. 11, p. 1292-1296. [CrossRef]
JALALI, R.; GHAFOURIAN, H.; ASEF, Y.; DAVARPANAH, S.J. and SEPEHR, S. Removal and recovery of lead using nonliving biomass of marine algae. Journal of Hazardous Materials, June 2002, vol. 92, no. 3, p. 253-262. [CrossRef]
JEON, Choong; YOO, Young Je and HOELL, Wolfgang H. Environmental effects and desorption characteristics on heavy metal removal using carboxylatedalginic acid. Bioresource Technology, January 2005, vol. 96, no. 1, p. 15-19. [CrossRef]
Anoop; VIRARAGHAVAN, Thiruvenkatachari and CULLIMORE, D. Roy. Removal
of heavy metals using the fungus Aspergillus
KESKINKAN, O.; GOKSU, M.Z.L.; BASIBUYUK, M. and FORSTER, C.F. Heavy metal adsorption properties of a submerged aquatic plant (Ceratophyllum demersum). Bioresource Technology, April 2004, vol. 92, no. 2, p. 197-200. [CrossRef]
MARTINS, Bruno L.; CRUZ, Claudio C.V.; LUNA, Aderval S. and HENRIQUES, Cristiane A. Sorption and desorption of Pb2+ ions by dead Sargassum sp. biomass. Biochemical Engineering Journal, January 2006, vol. 27, no. 3, p. 310-314. [CrossRef]
MATHEICKAL, Jose T. and YU, Qiming. Biosorption of lead from aqueous solution by marine algae Ecklonia radiata. Water Science and Technology, 1996a, vol. 34, no. 9, p. 1-7. [CrossRef]
Jose T. and YU, Qiming. Biosorption of lead from aqueous solution
by macro-fungi Phellinusbadius. In: Proceedings
of the 10th National Convention of Royal Australian Chemical
Institute. (27th September, 1996,
MATHEICKAL, Jose T. and YU, Qiming. Biosorption of lead(II) and copper(II) from aqueous solutions by pre-treated biomass of Australian marine algae. Bioresource Technology, September 1999, vol. 69, no. 3, p. 223-229. [CrossRef]
MURALEEDHARAN, T.R.; IYENGAR, L. and VENKOBACHAR, C. Screening of tropical wood-rotting mushrooms for copper biosorption. Applied and Environmental Microbiology, September 1995, vol. 61, no. 9, p. 3507-3508.
PADILHA, Flávia Pinto; DE FRANÇA, Francisca Pessôa and DA COSTA, Antonio Carlos Augusto. The use of waste biomass of Sargassum sp. for the biosorption of copper from simulated semiconductor effluents. Bioresource Technology, September 2005, vol. 96, no. 13, p. 1511-1517. [CrossRef]
Ofer; ARGAMAN, Yerachmiel and YANNAI, Shmuel. Mechanisms of biosorption
of different heavy metals by brown marine macroalgae.
SAG, Yesim; TATAR, Berya and KUTSAL, Tülin. Biosorption of Pb(II) and Cu(II) by activated sludge in batch and continuous-flow stirred reactors. Bioresource Technology, March 2003, vol. 87, no. 1, p. 27-33. [CrossRef]
SHENG, Ping Xin; TING, Yen-Peng; CHEN, J. Paul and HONG, Liang. Sorption of lead, copper, cadmium, zinc, and nickel by marine algal biomass: characterization of biosorptive capacity and investigation of mechanisms. Journal of Colloid and Interface Science, July 2004, vol. 275, no. 1, p. 131-141. [CrossRef]
VOLESKY, B.; WEBER, J. and PARK, J.M. Continuous-flow metal biosorption in a regenerable Sargassum column. Water Research, January 2003, vol. 37, no. 2, p. 297-306. [CrossRef]
Note: Electronic Journal of Biotechnology is not responsible if on-line references cited on manuscripts are not available any more after the date of publication.